Synthesis, Structure, and Bonding of the Zintl Phase Ba3Cd2Sb4
Bayrammurad Saparov; Sheng-qing Xia; Svilen Bobev; Inorganic Chemistry 47 (2008) 11237–11244; doi:10.1021/ic801530d

data_4306713
_publ_section_title
;
Synthesis, Structure, and Bonding of the Zintl Phase Ba3Cd2Sb4
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              11237
_journal_page_last               11244
_journal_paper_doi               10.1021/ic801530d
_journal_volume                  47
_journal_year                    2008
_chemical_formula_moiety         'Ba2.58 Cd2 Eu0.42 Sb4'
_chemical_formula_sum            'Ba2.58 Cd2 Eu0.42 Sb4'
_chemical_formula_weight         1129.96
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 111.6800(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   17.6492(16)
_cell_length_b                   4.8793(5)
_cell_length_c                   7.5676(7)
_cell_measurement_reflns_used    700
_cell_measurement_temperature    120(2)
_cell_measurement_theta_max      26.37
_cell_measurement_theta_min      2.48
_cell_volume                     605.59(10)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      120(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0201
_diffrn_reflns_av_sigmaI/netI    0.0148
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            3633
_diffrn_reflns_theta_full        26.37
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         2.48
_exptl_absorpt_coefficient_mu    22.525
_exptl_absorpt_correction_T_max  0.6742
_exptl_absorpt_correction_T_min  0.3096
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
; 
SADABS (Sheldrick, 2003) 
;
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.197
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             942
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.02
_refine_diff_density_max         0.682
_refine_diff_density_min         -0.806
_refine_diff_density_rms         0.214
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.126
_refine_ls_matrix_type           full
_refine_ls_number_parameters     30
_refine_ls_number_reflns         700
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.126
_refine_ls_R_factor_all          0.0159
_refine_ls_R_factor_gt           0.0146
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0191P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0348
_refine_ls_wR_factor_ref         0.0354
_reflns_number_gt                675
_reflns_number_total             700
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic801530d_si_002_4.cif
_cod_data_source_block           Ba3Cd2Sb4:Eu
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_database_code               4306713